 Nano Express
 Open Access
 Published:
Properties of Doped GaSb Whiskers at Low Temperatures
Nanoscale Research Letters volume 12, Article number: 156 (2017)
Abstract
Temperature dependencies of GaSb whiskers’ resistance doped with Te to concentration of 1.7 × 10^{18} cm^{−3} were measured in temperature range 1.5–300 K. At 4.2 K temperature, a sharp drop in the whisker resistance was found. The observed effect is likely connected with the contribution of two processes such as the electron localization in the whiskers and transition in superconducting state at temperature below 4.2 K. The whisker magnetoconductance is considered in the framework of weak antilocalization (WAL) model and connected with subsurface layers of the whiskers. The Shubnikovde Haas (SdH) oscillatory effect is observed in highquality ntype GaSb whiskers with tellurium doping concentration near the metalinsulator transition (MIT) for both longitudinal and transverse magnetoresistance.
Background
GaSb is an important material for practical implementation in microelectronic circuits, sensors, solidstate lasers, electrooptic modulators, and other new devices due to the high quality and perfection of single crystals [1, 2]. The GaSb epitaxial layers, or quantum dots grown on latticematched, semiinsulating substrates, are used in highspeed devices due to their advantages such as low density of dislocations and defects [3, 4]. However, these structures are affected by the substrate which restricts the advantages. Hence, GaSb single crystals [5] and freestanding nano and microwires [6] were used to avoid the abovementioned shortcoming. GaSb nanowires can also be used for lasing devices [7] that open the possibility of their applications for semiconductor subwavelengthwire lasers in photonic integrated circuits. The high charge carrier mobility and dimension dependence of conductance in GaSb∕GaAs nanowire heterostructures allow their wide usage [8, 9]. The highperformance GaSb nanowires could be integrated with devices on the base of InSb, InAs, and InGaAs nanowires by the various transfer techniques [8, 10].
Whiskers have several advantages over the wires, in particular, such as absence of defects due to the singlecrystal structure of whiskers caused by their growth conditions. Despite their large dimensions (as compared with nanowires), whiskers are important objects of nanoscale studies taking into account their coreshell structures [11]. New physical effects were obtained when the whiskers’ doping concentration corresponded to metalinsulator transition, for instance, giant piezoresistance effect in Si whiskers [12], appearance of magnetophonon oscillations in Ge whiskers [13], and giant spinorbit interaction with gfactor 60 in InSb whiskers [14]. However, GaSb whiskers were rarely studied from this point of view.
The aim of this work is to study spinorbit interaction for understanding observed superconductivity and weak antilocalization in ntype GaSb whiskers with Te impurity concentration near the metalinsulator transition by measurement of the magnetoresistance and magnetoconductance in the temperature range 1.5–300 K and magnetic field 0–14 T.
Methods
ntype GaSb whiskers doped with Te were selected for the study. The whiskers were grown by chemical vapor deposition (CVD) method in a closed system [15]. The whisker’s diameter ranges from 15 to 20 μm with length from 4 to 5 mm. Current electrical contacts were created by welding Pt whiskers on the opposite ends of the studied whiskers. The distance between potentiometric contacts was equidistant and equal to 1 mm. The method provides resistive contact to the samples in the temperature range 4.2–300 K. As a result, linear IV curves were obtained. Te is commonly used as ntype dopant in GaSb for creating the photovoltaic devices. The results of doped whiskers investigation by ion mass spectroscopy have shown that nGaSb whiskers (ρ_{300K} = 0.004 Ω cm) have Te concentration corresponding to the metallic side of metalinsulator transition and it is equal to 1.7 × 10^{18} cm^{−3}. To obtain reproducible results, a group of approximately ten whiskers with identical characteristics was studied. The samples have been cooled down to 1.5 K in helium cryostat. A special inset with a bifilar winding heater has been used to heatup samples to room temperature. Stabilized electrical current of 1–100 μA depending on the resistance of the sample has been generated by Keithley 224 current source. Digital multimeters Keithley 2000 and Keithley 2010, with simultaneous automatic data registration via parallel port of PC, have been used to measure both the voltage at potential contacts of the samples, output signals from thermocouple and magnetic field sensor with accuracy up to 1 × 10^{−6} V. The Bitter magnetbased setup has been used to study the effect of strong magnetic field on the samples. The induction of the magnet increases from B = 0 up to B = 14 T at a rate ~1.75 and 3.5 T/min at 4.2 K and higher temperature range, respectively.
Results
Temperature dependence of resistance for Tedoped GaSb whisker at a zero magnetic field is shown in Fig. 1 over the temperature range 1.5–300 K. Reviled R (T) with monotonic decrease of the resistance from 8 to 3.5 Ω in the temperature range 4.2–300 K corresponds to the metallic behavior of the electric resistivity of the GaSb whiskers. Unexpectedly the sudden decrease of GaSb whisker resistance from 3.5 to 3.25 Ω is observed at temperature just below 4.2 K. This interesting behavior of the resistance, namely, the sudden drop of R (T) at T ~4.2 K, could indicate the superconducting transition at this low temperature (inset in Fig. 1). To be sure, firstly, it should be discussed to what extent the junction properties (welded Pt microwires) influence the measurement data at about 4 K and may contribute to the observed drop in the resistance effect. To check the possible influence of Pt junctions, IV characteristics of the whiskers were measured in the temperature range 1.5–4.2 K. The measurements have shown that IV characteristics were linear at every fixed temperature and electrical contacts from Pt microwires remain ohmic. Thus, a sudden drop in the whisker’s resistance is hardly connected with influence of the Pt contacts at low temperatures.
On the other hand, the drop in resistance is very small, namely, about 8.6% ((3.5–3.2)/3.5 = 8.6%), and the resistance below 4 K is still very large in order to be interpreted as transition to the superconducting states, which expectedly is associated with a zero resistance. Nevertheless, one can suppose a presence of a small superconductive phase in the whisker. To support the idea, one can examine a diamagnetic response of GaSb<Te> whiskers below 4.2 K in small magnetic fields. Magnetization of GaSb whiskers versus magnetic field with strength from −1.5 up to 1.5 kOe at various fixed temperatures was measured using SQUID technics and presented in Fig. 2. As can be seen from Fig. 2, the hysteresis, being typical for type II superconducting state of GaSb whiskers, is observed in the available temperature range from 1.8 up to 4.2 K. The data in Fig. 2 allows estimation of critical values of H _{c1} and H _{c2}. All curves in Fig. 2 exhibit expected linear behavior at low fields (<250 Oe), which corresponds to the diamagnetic response of the sample. However, they deviate from the linearity at H _{c1}, which is expectedly different for different temperatures. Temperature dependence of H _{c1} is shown in the inset of Fig. 2 (curve 2). On the other hand, we can also estimate H _{c2} at the point where magnetic field intensity corresponds to zero magnetization (see arrow in Fig. 2). Estimated values of H _{c2} as a function of temperatures are shown in the inset of Fig. 2. As can be seen from the graph, the maximal H _{c2} value is approximately 750 Oe.
Thus, the partial superconducting transition of GaSb whisker is likely to occur at the critical temperature of about 4.2 K. Nevertheless, the reason of the superconductivity in the whiskers is not clear, since both the T _{c} = 1.09 K of Ga as well as the Curie temperature for GaSb<Te> is substantially lower. The possible reasons of the superconductivity in the whiskers could be their amorphization [16] or the heavy Te doping up to concentrations in the vicinity to metalinsulator transition, which is known to increase substantially the T _{c} values [17]. The amorphization of the GaSb whiskers is excluded as was observed in Shubnikovde Haas (SdH) oscillations, which are usually occurring in highquality crystals. Metallic phase in the vicinity to the localization threshold of metalinsulator transition (MIT) could be responsible for anomalous superconducting transition in GaSb crystals at temperatures near 4 K [18]. The other possible reason of partial superconductivity could be the creation of Sb_{2}Te_{3} nanoclusters, which are known to be topological insulators and to show a transition to superconducting state at T _{c} = 3 K [19]. However, Sb_{2}Te_{3} nanoclusters are unlikely to be created in the whiskers taking into account the relatively low Te concentration (1.7 × 10^{18} cm^{−3} according to data of mass spectroscopy investigation). As a result, the number of formed potential Sb_{2}Te_{3} nanoclusters is rather insufficient in order to provide the superconductive channel. Moreover, the partial superconductivity in the GaSb<Te> whiskers has been observed at T _{c} of about 4.2 K, which contradicts with T _{c} = 3 K observed for Sb_{2}Te_{3} inclusions.
Suppression of superconductivity by magnetic field is also informative for explaining its possible origin. In order to observe the influence of magnetic field on the resistivity drop below 4.2 K, one has to investigate the GaSb<Te> whiskers magnetoresistance R_{B}(T). Longitudinal and transverse magnetoresistance of ntype GaSb whiskers was studied in the temperature range 1.5–96 K and magnetic fields 0–14 T. Results of these investigations for GaSb whiskers with Te doping concentration 1.7 × 10^{18} cm^{−3}, which correspond to metallic side of the metalinsulator transition, are presented in Fig. 3. The oscillation peaks are distinctly seen on both longitudinal (H  to the transport current I) (Fig. 3a) and transverse (H ⊥ to I) (Fig. 3b) magnetoresistance at low temperatures (Fig. 3). Corresponding values of magnetic field induction at T = 4.2 K for both longitudinal and transverse magnetoresistance oscillation peaks are marked by arrows in the figure. The maximum peak amplitude expectedly decreases with the increase of the temperature in the whole range of applied fields. However, it is still observed up to at least 50 K.
Seven oscillation peaks were revealed on longitudinal R_{B}(B) dependence at liquid helium temperature (Fig. 3a). The number of transverse magnetoresistance peaks (Fig. 3b) decreases to four at 4.2 K in magnetic fields with induction up to 14 T. In our recent works, we found magnetophonon oscillations in nGe whiskers [13] and ShubnikovdeHaas (SdH) oscillations in nInSb whiskers in the temperature range 4.2–70 K [14]. In the present work, it is shown that the oscillations are observed in nGaSb whiskers in the low temperature range. The oscillations are attenuated with the increase of temperature and are already absent at temperatures above 60 K. This fact indicates that the observed oscillations can be attributed to SdH oscillations like those in InSb whiskers [14].
Next, we follow the welldeveloped methodology and construct the Landau fan diagram [20]. To do this, we assign a Landau level (LL) index number N to each resistance minimum (N + 1/2 to each resistance maximum) as shown in Fig. 3a, b by arrows. The Landau level index N versus reversal magnetic field induction 1/B (Landau fan diagram) is shown in the insets of Fig. 3a, b. As it is obvious from the insets of Fig. 3a, b, the data points fall on a straight line and the solid line represents the best linear fit. The intercept of the linear fit with the Nindex axis yields zero phase β = 0 that indicates in Schrodinger electron transport responsible for SdH oscillations.
Discussion
Magnetoresistance and Magnetoconductance of GaSb Whiskers in Low Magnetic Fields
Let us consider the influence of low magnetic fields on GaSb<Te> whisker resistance in the temperature range 4.2–1.5 K (Fig. 4). As can be seen from the figure, the longitudinal magnetoresistance dependencies demonstrate the expressed cusps at fields up to 1.0 T. To gain a deeper understanding of the physics associated with the superconductivity, we extracted the upper critical field B _{c} (T) (denoted by arrows in Fig. 4) from the magnetoresistance curves obtained at fixed temperatures. The obtained B _{c} (T) versus T/T _{c} dependence is shown in the inset of Fig. 4. Meanwhile, the value of the upper critical field at absolute zero temperature B _{c} (0) was obtained by fitting the data to the generalized GinzburgLandau model:
shown by the solid curve in the graph, where t = T/T _{c}.
Actually, the B _{c} (T) curve (inset of Fig. 4) exhibits a nearly linear dependence in the temperature range 1.5–4.2 K, as with topological YPtBi crystals [21]. Based on the linear dependence, the zero temperature upper critical field was obtained B _{c} (0) = 1.3 T by simple extrapolation (inset of Fig. 4, dash line).
The value of B _{c} (0) for GaSb is well below the Pauli paramagnetic limit:
which suggests an orbital pairbreaking mechanism of superconductivity for GaSb whiskers [21].
Using the relation:
where Φ_{0} is the flux quantum, we obtained superconductor coherence length ξ(0) = 1.7 nm. The obtained value is in good agreement with the coherence length ξ _{ab} (0) = 1.0 nm for cuprates [22].
The short coherence length (ξ(0) ~ 1.7 nm) of Cooper pairs, comparable with that found for highT _{c} superconductors, could lead to a variety of fascinating phenomena in contrast to lowT _{c} materials, which have homogeneous superconducting properties on length scales ξ _{0} of the order of several hundreds of nanometers [22]. Thus, the obtained low value of the coherence length is believed to provide an evidence for a possible competition of superconductivity and other physical phenomena in GaSb whiskers.
A small diminution of the whisker resistance (8.6%) at T ≤ 4.2 K suggests the formation of only small superconductive islands in the sample, which causes the observed partial transition of the whisker to the superconducting state. Since the main part of the whisker conductance is believed to occur on the whisker surface, like that in Si whiskers [12], one can suppose that the partial superconductivity of the whiskers should take place on their surface. However, if the sample is biphasic, the superconductive transition is expected to be somewhat blurred. That is why the obtained narrow transition (sudden drop of the resistance at T ≤ 4.2 K) just might be an additional argument in favor of the surface superconductivity in the whiskers.
It is worthy to note that the value of B _{c} (0) for GaSb, obtained from the above measurements, is an order of magnitude greater than the value obtained from magnetization measurement (of about 0.075 T). Thus, the obtained magnetoresistance cusps cannot be satisfactory explained only by the whisker transition to the superconducting state. Another possible reason of the whisker magnetoresistance cusps could be the effect of weak antilocalization (WAL) similar to that observed in the single crystals based on BiTe [23].
The nature of WAL can be caused by spinorbit interaction in the threedimensional bulk channel. However, in GaSb whiskers, the twodimensional nature of the electrical transports is assumed, as mentioned above, which is more likely to originate from the surface conductance, as it takes place in Si whiskers [12].
According to the WAL model [24], the electronelectron and electronphonon scattering are supposed to emerge in the whiskers. The theoretical dependence of normalized magnetoconductance Δσ(B)/G _{0} for twodimensional electron gas [24] has the following forms:
where B is the magnetic field induction and β is a factor determining the value of MakiThompson correction. Correspondingly,
is the quantum conductivity. Function f(x) is determined by the digamma function Ψ(z):
The parameter H _{ ϕ } is related with the dephasing time τ _{ ϕ } of the electron wave function caused by electronelectron or electronphonon interaction:
Accordingly, the parameter H _{ so } is related with the dephasing time τ _{ so } caused by spinorbit interaction of electrons:
where c is the light velocity and D is the diffusion coefficient.
Further, let us consider β → 0. In this case, the conductivity change Δσ(B) in a magnetic field, normalized by the amount G _{0}, was determined from experimental dependencies of GaSb whiskers’ magnetoresistance in magnetic field in the following way:
where μ is the Hall mobility and H is the magnetic field intensity. The temperature dependencies of the Hall mobility for GaSb whiskers were calculated in Ref. [25]. Thus, the obtained dependence Δσ(B) (Fig. 5) is matched with the theoretical one according to (4) in order to find the parameters H _{ ϕ } and H _{ so }. Figure 5 shows the magnetic field dependencies of normalized magnetoconductance change Δσ(B)/G _{0} of GaSb whisker at different temperatures (dots): 1–1.5, 2–3.3, 3–4.2, 4–12, 5–25, 6–42, and 7–50 K compared with theoretical curves calculated using (4) at the same temperatures (solid lines). As it is seen from Fig. 5, the very good coincidence of experimental data and theoretical curves is observed at low temperatures 1.5–50 K, when parameters H _{ ϕ } and H _{ so } are properly chosen. As mentioned above, obtained parameters H _{ ϕ } and H _{ so } depend on dephasing times τ _{ ϕ } (7) and τ _{ so } (8), respectively. The calculated values τ _{ ϕ } = 1 ps and τ _{ so } = 0.26 ps are similar to those reported in the literature [26]. The fact has to provide an evidence for the validity of the approach. The abovementioned parameters allow obtaining the coherence length L _{ ϕ } as well as the spinorbit length L _{ so } using the following relations:
From (10–11), the temperature dependencies of L _{ ϕ } and L _{ so } for the studied whiskers are calculated (Fig. 6).
It is well known that the coherence length L _{ ϕ } is proportional to T ^{− 1/3} for the onedimensional system and T ^{− 1/2} for the twodimensional one [27]. Figure 6 shows that coherence length L _{ ϕ } is proportional to T ^{− 0.53} and the spinorbit length L _{ so } to T ^{− 0.45}, which is very close to the T ^{− 1/2} dependence expected for the twodimensional system. This fact confirms the conclusion that conductance of GaSb whiskers mainly occurs in subsurface layers of the whiskers.
Therefore, weak antilocalization and superconductivity are the main possible mechanisms responsible for the magnetoresistance observation in GaSb<Te> whiskers that is likely to originate from the whisker surface.
Magnetoresistance Oscillations for GaSb Whiskers in High Magnetic Fields
We can analyze the whisker parameters also taking into account the SdH oscillations (Fig. 3). The magnetoresistance oscillations are periodic in 1/H. Magnetoresistance oscillation period P in the opposite field for quadratic dispersion law is described as follows [14]:
where e is the elementary charge, ℏ is the Planck constant, E _{ F } is the Fermi energy, m* is the effective cyclotron mass, and c is the speed of light. In the studied GaSb whiskers doped to Te concentration near the MIT, the period was found from experimental data and reaches 0.025 T^{−1}.
The analysis of SdH oscillations allows the finding of main GaSb whisker parameters. In particular, the cyclotron effective mass of electrons was determined according to the relative change in the amplitude of SdH oscillations at different temperatures A [14]:
where k _{B} is the Boltzmann constant.
This expression applies in the semiclassical region of fields assuming that it does not change with temperature and magnetic field. For weak magnetic fields, m _{ c } ≈ 0.047 m _{ o } is in good line with the literature data.
The mean free path of the charge carrier l _{ e } could be calculated based on the equation:
assuming a spherical Fermi surface with wave number:
The frequency of oscillation depends on the extreme section of the Fermi surface plane F = P ^{− 1} that is perpendicular to the magnetic field for an arbitrary dispersion law and shape of the Fermi surface, according to the relation:
The frequency of oscillation for longitudinal and transverse magnetoresistance coincides, which is in good agreement with the experimental results. Substituting F = P ^{− 1} in (16), one can calculate the Fermi surface S value. Taking the calculated value S = 3.8 × 10^{17} m^{−2} into account, we obtained the values of wave number k _{ F } = 3.46 × 10^{8} m^{−1} from (15) and mean free path of the charge carrier l _{ e } = 230 nm from (14).
Thus, l _{ e } > ξ, which confirms that GaSb is sufficiently pure to allow for oddparity superconductors. A comparison of free path of the charge carrier l _{ e } = 230 nm with phase coherence length L _{ ϕ } (Fig. 6) was shown to coincide in a wide temperature range 10–60 K. On the other side, the spinorbit length L _{ so } is shown to coincide with superconductance coherence length ξ that indicates the spinorbit origin of superconductivity.
According to D’yakonovPerel spin decoherence mechanism [28],
where d is the whisker diameter and L _{ Ω } is the spin processing length with Ω representing the spin processing frequency under spinorbit interaction. The spin processing length was calculated from the obtained data according to (17) and amounts to L _{ Ω } = 530 nm. Taking into account the equation
The Rashba spinorbit interaction parameter α was calculated and it is equal to α = 1.66 × 10^{−12} eV m which is in good line with literature data for GaSb nanowires 3 × 10^{−12} eV m [29]. A consequence of the emergence of large Rashba field is the possibility to polarize flowing electron along the direction of this field. As a result, magnetoresistance cusps are observed in longitudinal direction, while they are not appearing in transverse one at low magnetic fields (Fig. 3).
Substituting the value of wave number k _{ F } = 3.46 × 10^{8} m^{−1} and the Rashba spinorbit interaction parameter α in
, one can obtain the spin splitting energy Δ_{ so }, which was found to be Δ_{ so } = 1.15 meV for GaSb whiskers.
Thus, we can conclude that the experimentally observed WAL in GaSb whiskers is likely to result from the 2D surface conductivity channel of the whiskers. Due to the obtained large value of spin processing length L _{ Ω } = 530 nm, one could suppose that the superconducting nanoclusters are localized in subsurface layers of the GaSb whiskers.
In conclusion, one can return to the question about the nature of superconductivity in GaSb<Te> whiskers. The lower critical field H _{c1} shows clear linear temperature dependence from 4.2 down to 1.5 K (see inset in Fig. 2, curve 2), which could indicate a nonswave superconductivity but rather an unconventional superconductivity with a nodal gap structure [30]. A very low value of coherence length (ξ _{0} ~ 1.7 nm) like that of cuprates (ξ _{0} ~ 1 nm), as well as an unconventional nature of superconductivity in cuprates, could be connected with the similar features of these materials. Indeed, superconductivity of cuprates is underlined by the fact that these superconductors emerge from an antiferromagnetic Mott insulator upon carrier doping [31]. In the case of GaSb<Te> whiskers, weak antilocalization of charge carriers suggests antiferromagnetic correlation of the carriers in the metallic samples in the vicinity to MIT. The starting point is the Hubbard model in two dimensions from which we may derive an effective spin fluctuationbased interaction between electrons, which is eventually responsible for the formation of Cooper pairs. Thus, spin fluctuations could emerge due to the obtained large value of spinorbit interaction (spin processing length L _{ Ω } = 530 nm) and be responsible for competition between WAL and SC in GaSb whiskers.
Conclusions
The magnetoresistance of nGaSb whiskers with Te concentration 1.7 × 10^{18} cm^{−3}, near the metalinsulator transition, was studied in low temperature range from 1.5–96 K and magnetic fields with induction up to 14 T. Analysis of longitudinal and transverse magnetoresistance peaks allowed to identify them as the Shubnikovde Haas oscillations in the low temperature range 1.5–60 K. It was found that at T = 4.2 K, the number of transverse magnetoresistance peaks is smaller than the number of corresponding longitudinal magnetoresistance peaks.
Resistance of ntype GaSb whiskers was measured over the temperature range 1.5–300 K and magnetic field up to 10 T. The revealed sharp drop of resistance below 4.2 K indicates possible partial superconductivity in the whiskers. The magnetoconductance of these whiskers in lowfield regime can be well described by a twodimensional weak antilocalization model (WAL), where the dephasing length of the electrons follows T ^{− 1/2} dependence. Taking into account the WAL model as well as SdH oscillations analysis, the Rashba spinorbit interaction parameter α = 1.66 × 10^{−12} eV m was calculated. A consequence of the emergence of large Rashba field is the possibility to polarize flowing electrons along the direction of this field. As a result, magnetoresistance cusps are observed in longitudinal direction, while they are not appearing in transverse one. Due to the obtained large value of spin processing length L _{ Ω } = 530 nm and large whisker diameters (of about 20 μm), one can suppose that the superconductivity is created as a consequence of competition of superconductive and weak localized states in subsurface layers of the GaSb<Te> whiskers. The short coherence legnth (ξ (0) ~ 1.7 nm) of Cooper pairs serves as additional evidence of the competition of superconductivity and WAL in the whiskers. The origin of the superconducting state at temperature below 4.2 K is not clear, since the T _{c} = 1.09 K for Ga and the T _{c} = 3 K for possible Sb_{2}Te_{3} nanoclusters, as well as the Curie temperature for GaSb<Te>, are substantially lower. Appearance of superconductivity could be explained by strong spinorbit interaction of charge carriers in metallic phase in the vicinity to the localization threshold of MIT in the GaSb whiskers, which is known to increase substantially the Curie temperature. In order to confirm the abovementioned statement regarding the origin of the superconductive states, a thorough study of the whisker surface should be performed, which will be a task for the next investigations.
Abbreviations
 CVD:

Chemical vapor deposition
 LL:

Landau level
 MIT:

Metalinsulator transition
 PC:

Personal computer
 QDs:

Quantum dots
 SdH:

ShubnikovdeHaas
 SQUID:

Superconducting quantum interference device
 WAL:

Weak antilocalization
References
Fornari R, Roth Recent M (2009) Advances in bulk crystal growth. MRSBulletin 34(4):239–244
Rodriguez JB, Cerutti L, Tournie E (2009) GaSbbased, 2.2 μm typeI laser fabricated on GaAs substrate operating continuous wave at room temperature. Appl Phys Lett 94:023506
Richter J, Strassner J, Loeber T, Fouck H, Nowozin T (2014) GaSb quantum dots on GaAs with high localization energy of 710 meV and an emission wavelength of 1.3 μm. J Cryst Growth 404:48–53
Zhou W, Li X, Xia S, Yang J, Tang W, Lau K (2012) High hole mobility of GaSb relaxed epilayer grown on GaAs substrate by MOCVD through interfacial misfit dislocations. Array J Mater Sci Technol 28(2):132–136
Gadkari DB (2012) Advances of the vertical directional solidification technique for the growth of high quality GaSb. J Chem Chem Eng 6(1):65–73, http://www.davidpublishing.com/davidpublishing/upfile/5/1/2012/2012050186098929.pdf
Yang Z, Wang F, Han N, Lin H, Yuen Cheung H, Fang M, Yip S, Hung T (2013) Crystalline GaSb nanowires synthesized on amorphous substrates: from the formation mechanism to pchannel transistor applications. Appl Mater Interfaces 5:10946–10952
Chin H, Vaddiraju S, Maslov AV, Ning CZ, Sunkara MK, Meyyappan M (2006) Nearinfrared semiconductor subwavelengthwire lasers. Appl Phys Lett 88(16):163115
Guo YN, Zou J, Paladugu M, Wang H, Gao Q, Tan HH, Jagadish C (2006) Structural characteristics of GaSb∕GaAs nanowire heterostructures grown by metalorganic chemical vapor deposition. Appl Phys Lett 89:231917
Jeppsson M, Dick KA, Wagner JB, Caroff P, Deppert K, Samuelson L, Wernersson LE (2008) GaAs/GaSb nanowire heterostructures grown by MOVPE. J Cryst Growth 310:4115–4121
Ravi Kishore VV, Partoens B, Peeters FM (2012) Electronic structure of InAs/GaSb coreshell nanowires. Phys Rev B 86:165439
Klimovskaya AI, Prokopenko IV, Svechnikov SV, Cherneta TG, Oberemok A, Ostrovskii IP, Kurnosikov OV (2002) The structure, composition, and chemical state of the surface of wirelike silicon nanocrystal grown by selforganization technology. J P hys: Condens Matter 14(8):1735
Druzhinin A, Ostrovskii I, Khoverko Y, Koretskii R (2015) Straininduced effects in ptype Si whiskers at low temperatures. Mater Sci Semicond Process 40:766–771
Druzhinin AA, Ostrovskii IP, Khoverko YN, LiakhKaguy NS, Vuytsyk AM (2014) Low temperature characteristics of germanium whiskers. Funct Mater 21(2):130–136
Druzhinin A, Ostrovskii I, Khoverko Y, LiakhKaguy N, Khytruk I, Rogacki K (2015) Peculiarities of magnetoresistance in InSb whiskers at cryogenic temperatures. Mater Res Bull 72:324–330
Druzhinin AA, Ostrovskii IP (2004) Investigation of SiGe whiskers growth by CVD. Phys Stat Sol C 1(2):333–336
Demishev SV, Kosichkin YV, Sluchanko NE, Sharambeyan MS, Lyapin AG (1993) Crystallization of metastable phases and superconductivity in amorphous gallium antimonide. JETP 77(1):68, http://www.jetp.ac.ru/cgibin/dn/e_077_01_0068.pdf
Klein T, Achatz P, Kacmarcik J, Marcenat C, Gustafsson F, Marcus J, Bustarret E, Pernot J, Omnes F, Sernelius BE, Persson C, Ferreira da Silva A, Cytermann C (2007) Metalinsulator transition and superconductivity in borondoped diamond. PhysRev B 75:165313
Gantmakher VF, Zverev VN, Teplinskii VM, Tsydynzhapov GE, Barkalov OI (1993) Anomalous superconducting response and nonactivating tunneling in highresistance metastable states of GaSb. JETP 77(3):513, http://www.jetp.ac.ru/cgibin/dn/e_077_03_0513.pdf
Tsai WH, Chien CH, Lee PC, Ou MN, Harutyunyan SR, Chen YY (2016) Superconductivity and superconductorinsulator transition in single crystal Sb_{2}Te_{3} nanoflakes., http://www.mathpubs.com/detail/1608.05337v1/SuperconductivityandSuperconductorInsulatorTransitioninSingleCrystalSb2Te3Nanoflakes
Qu DX, Hor YS, Xiong J, Cava RJ, Ong NP (2010) Quantum oscillations and Hall anomaly of surface states in the topological insulator Bi2Te3. Science 329:821–824
Guizhou X, Wenhong W, Xiaoming Z, Yin D, Enke L, Shouguo W, et al (2014) Weak Antilocalization Effect and Noncentrosymmetric Superconductivity in a Topologically Nontrivial Semimetal LuPdBi. Scientific Reports 4
Tinkham M (1996) Introduction to superconductivity. McGrawHill, Inc., New York
Bao L et al (2012) Weak antilocalization and quantum oscillations of surface states in topological insulator Bi_{2}Se_{2}Te. Sci Rep 2:726
Bykanov DD, Novikov SV, Polyanskaya TA, Savel’ev IG (2002) Weak antilocalization and spinorbit interaction in a In0.53Ga0.47As/InP quantum well in the persistent photoconductivity state. Semiconductors 36(12):1389–1397
Druzhinin AA, Ostrovskii IP, Khoverko YN, Khytruk II (2015) The electron scattering on local potential of crystal defects in GaSb whiskers. J Nano Electron Phys 7(4):040841–040844, http://jnep.sumdu.edu.ua/uk/component/content/full_article/1677
Flatté ME, Byers JM, Lau WH (2002) Spin dynamics in semiconductors. In: Awschalom DD, Loss D, Samarth N (eds) Semiconductor spintronics and quantum computation. Springer, New York, pp 107–145. doi:10.1007/9783662050033_4
Altshuler BL, Aronov AG, Khmelnitsky DE (1982) Effects of electronelectron collisions with small energy transfers on quantum localisation. J Phys C: Solid State Phys 15:7367–7386
Kettemann S (2007) Dimensional control of antilocalization and spin relaxation in quantum wires. Phys Rev Lett 98(17):176808
Nimje S, Sharma A, Ghosh B (2015) Monte Carlo simulation of spin polarized transport in nanowires and 2D channels of III–V semiconductors. Quantum Matter 4(6):636–643
Wang XL, Dou SX, Ren ZA, Yi W, Li ZC, Zhao ZX, Lee SIK (2009) Unconventional superconductivity of NdFeAsO_{0.82}F_{0.18} indicated by the low temperature dependence of the lower critical field Hc_{1}. J Phys Condens Matter 21(20):205701
Mineev VP, Samokhin KV (1999) Introduction to unconventional superconductivity. Gordon &Breach Science Publishers, NewYork
Acknowledgements
The authors thank Prof. Solovjov A.L. (B.Verkin Institute for Low Temperature Physics and Engineering National Academy of Sciences of Ukraine) for the useful discussion of the experimental and theoretical results and Dr. Koreckii R.M. (Lviv Polytechnic National University) for the technical support and sample preparation.
Funding
No funding was received.
Authors’ Contributions
AD provided the technical support and conceptual advice; IK and IO analyzed and drafted the manuscript; YuK designed and conducted the experiments and performed the characterization of GaSb crystals; KR supported the experimental investigation; and NLK modified and drafted the manuscript. All authors have read and approved the final manuscript.
Competing Interests
The authors declare that they have no competing interests.
Declarations
This study has nothing to do with the human participants or healthrelated outcomes.
Author information
Authors and Affiliations
Corresponding author
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
About this article
Cite this article
Khytruk, I., Druzhinin, A., Ostrovskii, I. et al. Properties of Doped GaSb Whiskers at Low Temperatures. Nanoscale Res Lett 12, 156 (2017). https://doi.org/10.1186/s1167101719231
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/s1167101719231
Keywords
 Magnetoconductance
 ntype GaSb whiskers
 Weak antilocalization
 Superconductivity